Brief Survey of Wood Adhesives
By Carl A. Eckelman

Introduction
Adhesives may be defined as any substance capable of attachingmaterials together by means of surface attachment. This property is notnecessarily an intrinsic characteristic of the substance itself since theadhesive may be much weaker than the materials joined together, but it isdeveloped as the adhesive interacts with the adherends under certain
conditions of temperature and pressure.
Knowledge and use of adhesives is not new. The ancient Egyptians
knew well the art of veneering and used adhesives to attach decorations towood some 3500 years before Christ. Mud, dung, and clay, along with
mixtures of these substances, must also be regarded as adhesives and havebeen used for centuries to build huts in many parts of the world. Thatchedhuts plastered with a mixture of camel's dung and mud are still regularly
used in southwestern Saudi Arabia, for example.
Many types of glue have been used to bond wood together, but until
the time of the Second World War, essentially all of the glues were ofnatural origin. Adhesives based on synthetic polymers were introduced
just before WWII and now surpass most of the older natural glues inimportance for wood bonding. These synthetic adhesives are used insituations which are far too demanding for adhesives of natural origin andsatisfy moisture, durability, and strength requirements that were
unthinkable a few years ago. At one time, adhesives belonged exclusively
in the realm of the craftsmen; today, they have become indispensable tothe engineer as well.

Classification and Description
For the most part, adhesives used to bond wood together may beseparated into two distinct groups--those adhesives such as animal,
vegetable, casein, and blood glues which are formulated from materials ofnatural origin, and those adhesives which are based on synthetic resins
derived from petroleum, natural gas, and coal, i.e., products of thepetrochemical and related industries. The properties of various adhesives
are discussed below separated according to these two categories.Natural
Adhesives

Animal Glues
Animal glue was usually made from the hides and bones of suchanimals as cattle, horses, and sheep and was usually classified as either
hide or bone glue. Additional tissues such as sinews may also be used andsubstantial amounts of adhesive are made from fish. Animal glues may bepurchased as a powder, as beads, or as a jelly. The solid forms must be
soaked in water before they can be used. A good quality animal glue
should be able to soak up several times its weight in water and still remaina gelatinous mass. They are heated in glue pots to about 60° C (144° F) to
reduce their viscosity to a level where they can be applied. Some animalglues are sold in convenient liquid form, particularly the fish glues. Hot
animal glues develop an initial or tack strength on cooling but develop
their full strength only on drying. Animal glues have several shortcomings
which have lead to their replacement by other adhesives in a large part of
the woodworking industry. Specifically, they have low moistureresistance, are attacked by molds and fungi, are somewhat inconvenient touse and must be applied at the proper temperature, and are relatively
expensive. More importantly, there is strong competition for animal
remains today, and as a result animal glues are in short supply.
Capsule Summary•Form: Many grades sold in dry form; liquid glues available.
•Properties: High dry strength; low resistance to moisture and damp
conditions.
•Preparation and application: Dry form mixed with water, soaked, andmelted; solution kept warm during application; liquid forms applied asreceived; both pressed at room temperatures; adjustments in gluing
procedures must be made for even minor changes in temperature.
•Typical uses: Once widely used for furniture construction. Has largely
been displaced as an assembly glue by PVA's.

Starch Based Vegetable Glues
Although starch glues still are used in the United States, they are usedlittle in the wood industry. Of particular importance, they have been
replaced by urea-resin adhesives in gluing interior-type hardwood
plywood and furniture. They are included here largely as a matter ofhistorical interest.
As the name implies, the principal component of these adhesives isstarch which may be obtained from a variety of plants including corn,
potatoes, rice and cassava. The root of the cassava plant is the source oftapioca. Prior to World War II, extensive cassava plantations weremaintained by major glue companies in what is now Indonesia. During thewar, these plantations were lost, substitutes were found, and production ofglues which relied on this plant decreased accordingly. Vegetable glues
are ordinarily sold in powdered form and must be mixed with water. Otherchemicals such as alum may be added to improve their properties. These
mixtures are heated to prepare them for use--heating flour paste, forexample, renders the flour soluble. Vegetable glues are relatively
inexpensive and have a relatively long pot life. They set through loss ofwater, which may be quite slow, so that glued assemblies must often
remain clamped overnight. Vegetable glues were widely used during
World War I in such applications as veneering. They lack moistureresistance, however, stain certain veneer species, and are attacked by
micro-organisms.
Capsule Summary•Form: Mainly sold in dry form as flour.
•Properties: Produces tough dry bond; little resistance to moisture anddamp conditions.
•Preparation and application: Flour, water, and caustic are mixed andstirred with a brief cooking period. Mixture life relatively long.
•Typical uses: Primarily of historic interest. Formerly used in productionof plywood. Little used today.

Protein Based Adhesives
Soybean Glue
The principal protein-based vegetable glue is manufactured from either
soybean meal or the vegetable protein isolated from it. Soybean glue has
properties and characteristics which are similar to those of casein glue, butlacks its water resistance. Soybean glue may be hot-pressed, and in thepast was widely used for interior grade Douglas-fir plywood. Soybean
protein is also used in a blend, consisting primarily of blood and soybean
proteins. These are mixed and used like the hot-press blood glues.
Capsule Summary•Form: Protein sold in dry powder form (generally with small amounts ofdry chemical added) to be prepared for use by user.
•Properties: Moderate to low dry strength; moderate to low resistance towater and damp atmospheres; moderate resistance to intermediate
temperatures; white to tan in color.
•Preparation and application: Mixed with cold water, lime, caustic soda,
and other chemicals; applied and pressed at room temperatures, butmore frequently hot-pressed, especially when blended with blood
protein.
•Typical uses: Bonding softwood plywood for interior use. Now largely
displaced by phenolic resin in the softwood plywood industry.

Casein Glue
Casein glue is prepared from casein curd which is precipitated fromskim milk or buttermilk either by allowing the milk to sour naturally, or byadding acid to it. About eight gallons of skim milk are required to makeone pound of dry casein. To prepare the glue, the curds are dissolved in an
aqueous alkaline solvent such as lime water to which other chemicals suchas formaldehyde or copper chloride are added. Most casein glue is sold asa dry powder and must be mixed with water before it can be used. Once
mixed with water, casein glue has a relatively short pot life. Pot life can beincreased but only at the expense of moisture resistance. Until the
introduction of adhesives based on synthetic resins, casein glues were
important because of their superior moisture resistance. They are markedly
superior to animal and soybean glues in this respect. Casein glues haveseveral characteristics which limit their usefulness. They tend to stain
those species of wood which are rich in tannic acid such as the oaks, sothat casein glue is largely excluded from the furniture industry. They also
dull woodworking tools rapidly and are attacked by molds and fungi. In
recent years, casein glues have become expensive because of theincreasing needs for milk to feed the hungry of the world.
Capsule Summary•Form: Several brands sold in dry powder form; may also be preparedfrom raw materials by the user.
•Properties: Moderately high dry strength; moderate resistance to water,
damp atmospheres, and intermediate temperatures; not suitable forexterior uses; white to tan in color.
•Preparation and application: Mixed with water; applied and generallypressed at room temperature.
•Typical uses: Laminated timbers and doors for interior use.

Blood Glue
Blood-albumin glue is manufactured from whole blood which is a byproduct of slaughterhouse operations. Dried soluble blood powder is
produced by evaporating the serum from fresh whole blood. Bloodalbumin glue is then made by mixing the dried blood powder with waterand other chemicals such as lime and caustic soda.
Blood-albumin glues were, in a sense, forerunners of the synthetic
resins in that they required hot pressing in order to obtain proper setting
and curing of glue lines. In the dry state, blood-albumin glues havesomewhat less strength than the casein glues, but they are much superior
in moisture resistance. Until synthetic resins became generally available,
blood-albumin glues were the most important water resistant glues
available for plywood manufacture. They also showed moderate resistanceto intermediate temperatures and to micro-organisms. As a result, theseglues were widely used in the manufacture of plywood and still find someuse in that industry today. Older glues, referred to as "blood albuminglues," which were dispersed in ammoniacal water solutions for use as
hot-pressed plywood glues, are apparently used little in the United States.
Capsule Summary•Form: Primarily, dry soluble or partially insolubilized whole blood.
Commonly handled and used like soybean adhesives.
•Properties: Moderate resistance to water and damp atmospheres;moderate resistance to intermediate temperature and to microorganisms; dark red or black in color.
•Preparation and application: Mixed with cold water, lime, caustic soda,
and other chemicals; applied at room temperature and pressed either atroom temperature or in hot presses at 240° F or higher.

•Typical uses: Primarily for interior-type softwood plywood. Sometimes
in combination with soybean protein. Now largely displaced byphenolic resin.

Synthetic Resin Adhesives
Synthetic resins are man-made polymers which resemble natural resinsin physical characteristics but which can be tailored to meet specificwoodworking requirements. These resins impart to glue lines and joints
the highest water resistance attained to date. In contrast to the natural
adhesives which at best can resist only a moderate amount of moisture,properly formulated synthetic adhesives appear able to withstand repeateddirect wetting indefinitely. Synthetic resins were introduced aswoodworking adhesives during the early 1930's, but their greatest
development and use occurred during World War II, and their use is still
increasing today.
Synthetic resin adhesives may be separated into two distinct categories- thermosetting adhesives and thermoplastic adhesives. Thermosetting
adhesives depend upon a condensation type of polymerization reaction inwhich water is eliminated. During this cross linking reaction, the adhesive
undergoes an irreversible chemical and physical change which renders it
insoluble. The reaction itself may be initiated by means of chemicals orheat or a combination of both. Urea-formaldehyde, melamine
formaldehyde, phenol-formaldehyde, and resorcinol-formaldehyde alongwith phenol-resorcinol formaldehyde are included in this group ofadhesives. All of these resins utilize formaldehyde as a common raw
material.
Thermoplastic resins are prepolymerized and set by loss of dispersing
solvent. They do not undergo a chemical cross linking reaction whilecuring, therefore, but remain in a reversible state and can readily besoftened by heating. Polyvinyl acetate emulsions (white glue) and hot melt
glues belong to this group of adhesives.

Thermosetting Resins
Phenol-formaldehyde, the first of the synthetic resins to be developed,
was discovered by Dr. Leo Bakeland in 1909. Urea-formaldehyde,
resorcinol-formaldehyde, and melamine-formaldehyde were discovered
shortly thereafter. These products were already being considered foradhesive applications by 1920. Adhesives based on phenol-formaldehyde
and resorcinol-formaldehyde resins were well established by 1940 and as
previously noted, were widely used during World War II.

Urea-Formaldehyde
Urea-formaldehyde resins are probably the most widely used
thermosetting resin for wood. They are widely used for the manufacture ofinterior grade plywood and also for the manufacture of particleboard. In
particular, they are extensively used in producing hardwood plywood for
furniture and interior paneling and for furniture assembly. They areavailable in both liquid and powder forms and may be mixed with

hardeners, fillers, and extenders to obtain formulations which cure attemperatures ranging from room temperature to nearly 400o F. Fillers andextenders are added to the resin to control flow, viscosity, resin
penetration into the wood, and to lower glue line costs. Unmodified ureaformaldehyde resins are light colored and form joints which have highmoisture resistance. Extension of these resins with various flours
significantly reduces their moisture resistance. Urea-formaldehyde resins
may also be fortified with melamine resins to improve both their moistureand temperature resistance.
Capsule Summary•Form: Many brands sold as dry powders; others as liquids; may be
blended with melamine or other resins.
•Properties: High in wet and dry strength moderately durable under damp
conditions; moderate to low resistance to temperatures in excess of
120° F; white or tan in color.
•Preparation and application: Dry form mixed with water; hardeners,
fillers, and extenders may be added by user to either dry or liquid
form; applied at room temperatures; some formulas cure at room
temperatures; other require hot pressing at 210° to 250° F.
•Typical uses: Hardwood plywood for interior use and furniture; interior
particleboard; underlayment, flush doors, furniture core stock.

Melamine-Formaldehyde
Melamine resins are used primarily to improve the moisture resistanceof urea-resin adhesives. In this respect, they are substantially moreresistant than urea-resins but not as resistant as phenol and resorcinol
resins. Melamine resins must be cured at temperatures of at least 240° F
for most applications. They are also quite expensive relative to the urearesins. These two factors have limited the use of straight melamine-resins
to a few special applications such as marine plywood where the need for alight-colored water-resistant adhesive justifies their cost.
Capsule Summary•Form: Comparatively few brands available; usually marketed as apowder with or without catalyst.
•Properties: High in both wet and dry strength; very resistant to moistureand damp conditions depending on type and amount of catalyst; white
to tan in color.
•Preparation and application: Mixed with water and applied at room
temperature; temperatures of 250° to 300° F. required to cure.
•Typical uses: Primarily a fortifier for urea resins for hardwood plywood,end-jointing and edge-gluing of lumber, and scarf joining softwood
plywood. High-frequency cure compatible.

Phenol-Formaldehyde
Phenol-formaldehyde resins are widely used to produce softwood
plywood for severe service conditions. These resins are dark reddish incolor and are available as liquids and powders or in film form. They may
be manufactured to cure at a variety of temperatures ranging from room
temperature to over 275° F. When compounded with fillers andaccelerators, they still produce joints which exhibit high bond strength
even under severe conditions of exposure. Their use is almost mandatory
in plywood to be used in severe service conditions. Most types used in the
United States are alkaline-catalyzed. Acid-catalyzed systems are alsoavailable, primarily for use at curing temperatures of 70° to 140° F, but
are used little in the United States. Principal limitation is the possible
damage to wood by the acid catalyst.
Capsule Summary•Form: Many brands available, some dry powders, others as liquids, andat least one as dry film. Most commonly sold as aqueous, alkalinedispersions for plywood, and as powder or liquid for waferboard and
OSB manufacture.
•Properties: High in both wet and dry strength; very resistant to moistureand damp conditions, more resistant than wood to high temperature;often combined with neoprene, polyvinyl butyral, nitrile rubber, or
epoxy resins for bonding metals. More resistant than wood to chemical
aging; dark red in color.
•Preparation and application: Film form used as received; powder form
mixed with solvent, often alcohol and water, at room temperature; withliquid forms, modifiers and fillers are added by users; most common
types require hot-pressing at about 260° to 300° F. Temperatures ashigh as 400° F may be used for structural composites.
•Typical uses: Primary adhesive for exterior softwood plywood andflakeboard.

Resorcinol and Phenol-Resorcinol Formaldehyde
These glues are more expensive than the straight phenol-formaldehyde
resins and are used primarily as special purpose adhesives. They are dark
reddish in color and are generally supplied in liquid form. A filled liquidor powdered hardener is added to the liquid prior to use. Curing
temperatures range from 70° to 150° F. Because of their cost, resorcinol
based adhesives are not widely used for plywood manufacture; rather, they
are used as assembly glues in solid wood products which must resist
exposure to the weather and to water such as glued laminated wood beams
and I-joists. They have been of particular value in a few unique exacting
applications such as the manufacture of wood aircraft.
Capsule Summary•Form: Several brands available in liquid form; hardeners supplied
separately; some brands are combinations of phenol and resorcinol
resins.
•Properties: High in both wet and dry strength; very resistant to moistureand damp conditions; more resistant than wood to high temperatureand chemical aging; dark red in color.
•Preparation and application: Mixed with hardener and applied at room
temperatures; resorcinol adhesives cure at room temperatures on most

species; phenol-resorcinols cure at temperatures form 70° to 150° F,
depending on curing period and species.
•Typical uses: Primary adhesives for laminated timbers and assembly
joints that must withstand severe service conditions.

Isocyanates
Isocyanate based adhesives were first used in the 1940's, but their highcost, along with technical difficulties and associated health hazards,
largely prevented their commercial application. Technical improvements,
along with the demand for board products which are totally free offormaldehyde emissions, subsequently lead to the use of isocyanate
binders for particleboard manufacture. Isocyanate particleboard has been
manufactured in Germany since 1975 and is being used increasingly in the
U.S. today. It has excellent resistance to moisture and hence is well-suitedfor exterior applications. In addition to wood, isocyanates may also be
used to bond agricultural cellulosic wastes such as straw and bagasse.
Isocyanates may also be used as assembly glues, but the cost of theadhesive limits their use at the present time.
The basic bonding mechanism consists of forming urethane bridges
with the hydroxyl groups of the cellulose. This results in an extremely
strong wood to adhesive bond which is resistant to moisture as well as
dilute acids (Pizzi, 1963).
Capsule Summary•Form: Liquid resins or water emulsions or with other resins to form
polyurethane adhesives. Great versatility in formulating wide varietyof adhesives; some forms may give toxic vapors.
•Properties: Excellent adhesion to wood and many other materials.
Resistance to moisture and elevated temperature varies widely;
excellent chemical aging resistance.
•Preparation and application: One-part adhesives cure on application ofheat or in presence of moisture; two-part resins cure upon mixing ateither room temperature or elevated temperature; very rapid cures are
possible.
•Typical uses: Limited use in structural flakeboard , film laminating, andas an assembly adhesive; use has been limited by high relative cost andin some instances by sensitivity to heat and moisture.

Thermoplastic Resin Adhesives
Polyvinyl Acetates
Polyvinyl acetate adhesives--the common white glues seen in both
drug stores and furniture factories--have become one of the mostimportant assembly glues in the woodworking industry. They are
ordinarily sold as a ready-to-use aqueous emulsion in which the amount of
resin present is specified in percent. These resins set rapidly at room
temperatures and have high dry strength, but their moisture resistance isinferior to that of the urea-formaldehyde resins; furthermore, joints withthick glue lines tend to creep under sustained loads. They also have poor

resistance to heat. Modified vinyl-resin emulsions are available, however,which involve addition of a curing agent at time of use, resulting in greatly
improved resistance to heat and moisture.
Because of their ease of application, their high dry strength, the factthat they can be used with low clamping pressures (although joints ofquestionable quality may result) and their competitive cost, polyvinyl
acetate adhesives are widely used for furniture assembly and have nearly
displaced all other glues for this purpose.
Capsule Summary•Form: Several brands are available , varying to some extent in properties;
often copolymerized with other polymers; marketed in liquid form
ready to use.
•Properties: Generally high in dry strength; low resistance to moisture andelevated temperature; joints tend to yield under continued stress; whiteor yellow in color.
•Preparation and application: Ready to use liquid; applied and pressed atroom temperature.
•Typical uses: Furniture assembly, flush doors, bonding plastic laminates.
Assembly of manufactured homes for transportation shock resistance.

Hot Melt Adhesives
Hot melt adhesives are resins which are normally solid but melt uponheating so that they may be applied as a drop or a bead of glue. Upon
cooling, they immediately regain their adhesive properties. Ordinarily, hotmelts are not used in structural applications where high strength isrequired but rather, are commonly used to attach decorative materials suchas edge banding to panels and table tops. The adhesives themselves are
based on various polymers including the polyolefins, the vinyl
acetateolefin copolymers, polyamides, and the polyurethanes.
Capsule Summary•Form: Solid chunks, pellets, ribbons, rods, or films; solvent-free.
•Properties: Rapid bonding; gap-filling; lower strength than conventional
wood adhesives; minimal penetration; moisture resistant; white to tan
in color.
•Preparation and application: Melted for spreading; bond formulation bycooling and solidification; requires special equipment for controllingbonding conditions.
•Typical uses: edge banding of panels; plastic lamination; patching; films
and paper overlays; furniture assembly.

References for Further Reading
Anon. 1977 Adhesives Used in the Wood Processing Industries. ID/223(ID/WG.248/17) UNIDO 27 pp.
FPL. 1978. Adhesives in Building Construction. USDA Handbook No.
516. 160 pp. USGPO. Wash.
Pizzi, A. 1983. Wood Adhesives. Marcel Dekker, Inc. New York. 364 pp.

Reinhardt, J. 1974 Adhesives for Wood. (Plus one page summary).
ID/WG.200/3 UNIDO 28 pp.
USDA Forest Service, Forest Products Laboratory. 1987. Wood
Handbook: Wood as an Engineering Material. Agric. Handb. 72.
USGPO. Wash., DC.

References of Historical Value
Anon. 1951. Wood Aircraft Inspection and Fabrication. ANC-19.335 pp.
Superintendent of Documents. USGPO. Wash., DC.
Blakeland, L.H. 1909. Ind. Eng. Chm. Vol. 1, p. 149.
_________________1913. Ind. Eng. Chm. Vol. 5, p. 506.
FPL. June, 1955. Animal Glues: Their manufacture, Testing, andPreparation. FPL Rept. No. 492. 13 pp.
___. May, 1959. Blood Albumin Glues: Their Manufacture, Preparation,
and Application. FPL Rept. No. 281-2. 5 pp.
___. March, 1956. Casein Glues: Their Manufacture, Preparation, andApplication. FPL Rept. No. 280. 12 pp.
___. April, 1959. Synthetic-Resin Glues. FPL Rept. No. 1336. 25 pp.
___. October, 1955. Vegetable (Starch) Glues. FPL Rept. No. 30. 10 pp.
Perry, Thomas D. 1944. Modern Wood Adhesives. 208 pp. Pitman
publishing Corp., New York.
______________ 1948. Modern Plywood. 2nd ed. 458 pp. Pitman
Publishing Corp., New York.
Knight, R.A.G. 1952. Adhesives for Wood. 242 pp. Chemical PublishingCo., New York.